Synthesis of cobalt nanoparticles on Si (100) by swift heavy ion irradiation
© Attri et al.; licensee Springer. 2013
Received: 28 August 2013
Accepted: 7 October 2013
Published: 18 October 2013
We report the growth and characterization of uniform-sized nanoparticles of cobalt on n-type silicon (100) substrates by swift heavy ion (SHI) irradiation. The Co thin films of 25-nm thicknesses were grown by e-beam evaporation and irradiated with two different types of ions, 45-MeV Li3+ and 100-MeV O7+ ions with fluences ranging from 1 × 1011 to 1 × 1013 ions/cm2. SHI irradiation, with the beam rastered over the area of the film, resulted in the restructuring of the film into a dense array of Co nanostructures. Surface topography studied by atomic force microscopy revealed narrowed size distributions, with particle sizes ranging from 20 to 50 nm, formed through a self-organized process. Ion fluence-dependent changes in crystallinity of the Co nanostructures were determined by glancing angle X-ray diffraction. Rutherford backscattering spectroscopy analysis showed the absence of beam-induced mixing in this system. Surface restructuring and beam-induced crystallization are the dominant effects, with the nanoparticle size and density being dependent on the ion fluence. Results are analyzed in the context of molecular dynamics calculations of electron-lattice energy transfer.
KeywordsCobalt nanostructures Ion irradiation Surface restructuring Atomic force microscopy Thin films
The synthesis of metallic nanoparticles from thin films offers the possibility of scientific insight into novel processes  as well as advantages in development due to the adaptation of existing thin film technology. Potential applications range from nanostructured magnetic media  to catalysts in energy conversion and templates for the growth of semiconductor nanowires and CNTs . Apart from this, the plasmonic resonance in metal nanoparticles is extremely sensitive to changes in the surroundings, making them suitable for biosensing, with diagnostic and therapeutic applications being developed . Today, these materials are being synthesized and modified by various physical and chemical methods. However, the synthesis of size-controlled nanoparticles remains a challenge, and many new methods are being explored. Restructuring of thin films of a few tens of nanometer thickness is one such route, which has been undertaken for a wide range of materials, with films being fabricated in various ways, viz., sol–gel, spin coating , RF magnetron sputtering, pulsed laser deposition (PLD) , and electron beam evaporation . Post-growth processing has been broadly categorized into two - thermal treatment and irradiation by particle beams. The former method involves uniform heating in vacuum  or laser beam irradiation resulting in either uniform heating or variable heating through the creation of thermal distribution patterns on the surface by interference of laser beams . The particle beam treatment may range from the use of ion beams of a few keV from lab ion guns  to high-energy beams with hundreds of MeV available from ion beam particle accelerators [11, 12].
Highly focused ion beam (FIB) systems offer excellent control and the possibility of 'sculpture’ on the nanoscale, but such top-down methods suffer from limitations of time, scalability, and wastage of resources . Ion beam irradiation is a unique tool for engineering nanoparticles as it provides the possibility of both 'top-down’ and 'bottom-up’ mechanisms to produce nanoparticles of uniform sizes, using the intrinsic properties of the metals and metal-substrate interfaces. As the incident ion passes through a solid, energy is lost via interactions with target nuclei (nuclear energy loss (Sn)) and target electrons (electronic energy loss (Se)) . In the low-energy ion irradiation regime (up to a few tens of keV), collisions with target nuclei are significant, with atomic displacements and recoiled target atoms yielding collision cascades. Upon irradiation by what are called swift heavy ions (SHI; or ions of masses greater than H and He, with energies in the MeV region), electronic energy loss is dominant, with ionization along the ion track and significant energy transfer to the electrons of the target. This energy is then transferred to the lattice, resulting in a 'thermal spike,’ as the kinetic energy of the atoms along the ion track goes up dramatically for a few fractions of a picosecond following the ion transit. This could lead to significant atom displacement and mass movement, even to the surface . The resulting changes in the target depend on the systems being considered (ion mass as compared to the target, ionic charge, incident energy, and the electronic structure of the target - whether metal, semiconductor, or insulator), varying from amorphization to crystallization and shape change of implanted targets in the direction of the ion beam [15, 16]. In the case of metal films, due to the delocalized electronic configuration, models of energy transfer have had to consider electronic thermal spike effects as well [17–19].
Co nanoparticles are important due to crystallite size-dependent magnetic properties and site-selective catalytic activity [19, 20]. Some irradiation studies on the same Co/Si (100) system have been reported in the literature, with results that vary considerably depending on the identity and energy of the incident ions. Lian et al.  used a 25-keV FIB beam for initial processing to form strips of various widths and then rastered the defocused beam across the film, resulting in sputtering and dewetting of the film, driven by the Rayleigh instability . Agarwal et al.  have found silicide formation at the interface of the Co/Si system upon irradiation with much heavier Au ions of 120 MeV. Mixing at the interface has also been reported with this system [22, 23], with Rutherford backscattering spectroscopy (RBS) being used to quantify the changes observed.
Our work is an effort to characterize the change in morphology observed upon irradiation with ions of different masses and incident energies, and the effect of ion fluence on the development of nanoparticles so as to gain insight into the mechanism by which such large-scale atom movement occurs.
The samples were prepared at the Target Lab of the Inter University Accelerator Centre, New Delhi (IUAC). A Co thin film of 25-nm thickness was deposited on n-type silicon (100) substrates with a size of approximately 1 × 1 cm2 (scored and cut from commercial wafers and cleaned by sonicating in warm acetone and methanol) by e-beam evaporation at room temperature. Vacuum during deposition was maintained at approximately 7 × 10-7 mbar, and a quartz crystal monitor was used to monitor the thickness of the deposited film. These films were later irradiated with ions from the 15 UD Pelletron accelerator at the IUAC. In order to characterize the ion type, energy, and fluence required for nanostructure formation, these films were bombarded with Li3+ and O7+ beams, having an energy of 45 and 100 MeV, respectively. For both sets of ions, the samples were irradiated with five different fluences, i.e., 1 × 1011, 5 × 1011, 1 × 1012, 5 × 1012, and 1 × 1013 ions/cm2. We present data from three sets of fluences, i.e., 1 × 1011, 1 × 1012, and 1 × 1013 ions/cm2, for clarity.
When the energetic ions collide with the target atoms of the deposited Co film, there are two types of energy loss mechanisms - nuclear energy loss (dominant in the keV energy range) and electronic energy loss (which is dominant in the MeV energy range). In our experiment, 45-MeV Li3+ and 100-MeV O7+ ions have nuclear energy loss of 0.1762 and 1.224 keV/μm, respectively, and electronic energy loss of 3.098 × 102 and 2.076 × 103 keV/μm, respectively. Li3+ and O7+ ions have projected ranges of 88.95 and 34.10 μm, respectively in Co/Si. Thus, the loss mechanism in the given energy range is dominated by electronic energy loss in both cases, but the loss in the case of oxygen ions is about seven times higher, allowing for a comparative study. As mentioned above, reports in the literature also indicate that the mass of the ion has a significant effect on the consequences of ion bombardment [21–23]. The above parameters were obtained on the basis of SRIM-2008 calculations .
Surface structure and roughness were analyzed by atomic force microscopy (Nanoscope IIIa (Veeco, Santa Barbara, CA, USA) at the Material Science Group, IUAC) in the tapping mode with an antimony-doped silicon tip. The crystal structure is studied by X-ray diffraction (XRD) carried out using a PW3710 diffractometer (Phillips, Eindhoven, Netherlands; at the Crystal Growth Laboratory, Department of Physics, Jamia Millia Islamia, New Delhi) with nickel-filtered Cu Kα (λ = 1.5418 Å); the sample was scanned over 10° to 80° at the rate of 2°/min. The composition of the as-deposited and irradiated samples is measured by Rutherford back scattering spectroscopy (RBS) using a He+ beam of 2-MeV energy at the Inter University Accelerator Centre .
Results and discussion
As irradiation proceeds, uniformly distributed nanoparticles develop, with increasing number density (particles per unit area) as fluence is increased. The grain size distribution is found to narrow with increase in ion fluence, and the shape of the grains also appears to be more well defined and uniform at the highest fluence used (see Figures 1b,c,d). Surface roughness (defined as rms deviation from the mean surface height) initially increases from a value of 0.214 nm for the pristine film to 0.650 nm for our initial fluence of 1 × 1011 ions/cm2, due to the perturbations that are created as the ions impinge on the surface. At this fluence, only 1 in 1,000 atoms on the surface has undergone a collision with an incident ion. As irradiation proceeds, a higher fraction of surface atoms is bombarded and the density of perturbed regions of the film increases and the roughness decreases until the lowest value of 0.429 nm is reached, for a fluence of 1 × 1013 ions/cm2. This roughness value is still twice that of the pristine surface, indicating the transformation that has taken place. The reduction in roughness has also been reported by Lian et al.  as a 'nanosmoothing’ process.
In Figure 2b, the topography indicates that upon irradiation with the Li3+ beam, the nanostructures obtained are not as well defined as with the oxygen beam. The size distribution also peaks at a higher value of about 50 nm, as compared to the case of the O7+ beam.
The structural modification of the Co/Si (100) system under 100-MeV oxygen and 45-MeV lithium ions has been examined by XRD. Spectra for pristine and irradiated samples are shown in Figure 4.
The pristine sample shows two peaks at 44.77° and 52.01° which are identified as cobalt (111) and (200), from the JCPDS database (JCPDS 15–0806). After irradiation with 100-MeV oxygen ions, the peak intensity increases sharply, with the increase being maximum for the lowest fluence studied. The increment in the (111) peak is seen to be more than that of the (200) peak. As SHI irradiation helps to release the strain by local heating of the film, this could be responsible for the initial improvement in crystallinity. When the film is irradiated with Li3+ ion at lower fluence (1 × 1011 ion/cm2), the Co peaks disappear, but the (200) peak reappears upon further irradiation at the fluences of 1 × 1012 and 1 × 1013 ions/cm2 (at the angle of 52.01°). The clear variation in the beam-induced effects with different ions suggest that the mechanism for the changes in crystallinity of the films depends on the specific energy and identity of the bombarding ions and can only be determined following detailed simulations of this system, as initiated in the molecular dynamics calculations reported by Mookerjee et al. . Their calculations indicate the rapid quenching of the instantaneous temperature spike (up to thousands of degrees Kelvin) in the sub-picosecond time scale, so the possibility of nanoscale melting and recrystallization must be considered .
Results obtained from our studies show that the synthesis of cobalt nanoparticles is strongly dependent on the mass and energy of the incident ions. AFM scans reveal that nanoislands of cobalt are formed on the n-silicon (100) surface when irradiated both with oxygen and lithium ions, but the details of the morphology obtained differ in each case. XRD analysis shows some changes in crystallinity of the Co but no evidence of silicide formation at the interface.
In the present case, the mechanism of formation of Co nanoparticles on the substrate follows from the thermal spike model  which suggests that a transient nanoscale local hot molten zone of several thousands of degrees Kelvin is formed along the ion track through the film. Within the picosecond time frame, the track cools down and agglomerates of metal nanoparticles are formed. Sprouster et al. reported 120-MeV Au ion-induced transformation of shape in embedded Co nanoparticles above a threshold size parallel to the incident ion directions . In their case, the shape transformation is constrained by the matrix within which the Co particles are placed. In the case of metallic thin films deposited on substrates, the surface energy mismatch drives the transformation due to the local heating and leads to atomic displacement and the eventual coalescence of the film into nanoscale structures.
Cobalt nanoparticles were synthesized on a silicon (100) wafer by SHI irradiation, with 45-MeV Li3+ and 100-MeV O7+ ions, at room temperature. AFM studies showed the formation of globule-shaped cobalt nanoparticles on the surface of the film. Characterization by RBS and XRD studies suggests that the crystallinity of the Co is increased and that no silicide formation was detected in our experiment. The present study suggests that SHI-induced irradiation is a promising way to grow nanoparticles from thin films through a self-organized process and that this approach enables size-controlled production of uniformly distributed nanoparticles.
Atomic force microscopy
Focused ion beam
Rutherford backscattering spectroscopy
Swift heavy ion
The first author is thankful to the University Grants Commission for providing the fellowship, to Sristi and Hasmuddin for characterization with AFM and XRD, respectively, and to Phanendra for discussions. All authors gratefully acknowledge the support of the Target Lab, the Pelletron Group, and the Materials Group at the Inter University Accelerator Center, New Delhi.
- Lian J, Wang L, Sun X, Yu Q, Ewing RC: Patterning metallic nanostructures by ion-beam-induced dewetting and Rayleigh instability. Nano Lett 2006, 6: 1047–1052. doi:10.1021/nl060492z 10.1021/nl060492zView Article
- Huttel Y, Gómez H, Clavero C, Cebollada A, Armelles G, Navarro E, Ciria M, Benito L, Arnaudas JI, Kellock AJ: Cobalt nanoparticles deposited and embedded in AlN: magnetic, magneto-optical, and morphological properties. In J Appl Phys 2004, 96: 1666–1673. doi:10.1063/1.1767975 10.1063/1.1767975View Article
- Bischof J, Scherer D, Herminghaus S, Leiderer P: Dewetting modes of thin metallic films: nucleation of holes and spinodal dewetting. Phys Rev Lett 1996, 77: 1536–1539. doi:10.1103/PhysRevLett.77.1536 doi:10.1103/PhysRevLett.77.1536 10.1103/PhysRevLett.77.1536View Article
- Khenner M, Yadavali S, Kalyanaraman R: Formation of organized nanostructures from unstable bilayers of thin metallic liquids. Phys Fluids 2011, 23: 122105–122118. doi:10.1063/1.3665618 10.1063/1.3665618View Article
- Lu F, Tennyson DL, Zhu J-J, Burda C: Gold nanoparticles for diagnostic sensing and therapy. Inorg Chim Acta 2012, 393: 142–153. doi:10.1016/j.ica.2012.05.038View Article
- Doria G, Conde J, Veigas B, Giestas L, Almeida CM, Assunção M, Rosa J, Baptista PV: Noble metal nanoparticles for biosensing applications. Sensors 2012, 12: 1657–1687. doi:10.3390/s120201657 10.3390/s120201657View Article
- Rath H, Dash P, Som T, Satyam PV, Singh UP, Kulriya PK, Kanjilal D, Avasthi DK, Mishra NC: Structural evolution of TiO2 nanocrystalline thin films by thermal annealing and swift heavy ion irradiation. J Appl Phys 2009, 105: 074311–074316. doi:10.1063/1.3103333 10.1063/1.3103333View Article
- Lebedev DV, Ziganshina SA, Nurgazizov NI, Chuklanov AP, Bukharaev AA: Formation of Co nanoparticles on a pyrolytic graphite surface in ultrahigh vacuum. J Surface Investig X-ray Synchrotron Neutron Tech 2012, 6: 541–545. doi:10.1134/s1027451012060183 10.1134/S1027451012060183View Article
- Favazza C, Kalyanaraman R, Sureshkumar R: Robust nanopatterning by laser-induced dewetting of metal nanofilms. Nanotechnology 2006, 17: 4229. doi:10.1088/0957-4484/17/16/038 10.1088/0957-4484/17/16/038View Article
- Hua X, Cahill DG, Averback RS: Nanoscale pattern formation in Pt thin films due to ion-beam-induced dewetting. Appl Phys Lett 2000, 76: 3215–3218. doi:10.1063/1.126633 10.1063/1.126633View Article
- Bolse TA, Elsanousi H, Paulus W, Bolse W: Dewetting of nickel oxide films on silicon under swift heavy ion irradiation. Nucl Instrum Meth in Phys Res B 2006, 244: 115–119. doi:10.1016/j.nimb.2005.11.053 10.1016/j.nimb.2005.11.053View Article
- Krasheninnikov AV, Nordlund K: Ion and electron irradiation-induced effects in nanostructured materials. J Appl Phys 2010, 107: 071301–071370. doi:10.1063/1.3318261 10.1063/1.3318261View Article
- Avasthi DK, Pivin JC: Ion beam for synthesis and modification of nanostructures. Curr Sci 2010, 98: 780–792.
- Bringa EM, Johnson RE: Coulomb explosion and thermal spikes. Phys Rev Lett 2002, 88: 165501–165504. doi: 10.1103/PhysRevLett.88.165501View Article
- Dawi EA, Vredenberg AM, Rizza G, Toulemonde M: Ion-induced elongation of gold nanoparticles in silica by irradiation with Ag and Cu swift heavy ions: track radius and energy loss threshold. Nanotechnology 2011, 27: 215607–215611. doi:10.1088/0957-4484/22/21/215607View Article
- Kumar H, Ghosh S, Avasthi DK, Kabiraj D, Mücklich A, Zhou S, Schmidt H, Stoquert J-P: Ion beam-induced shaping of Ni nanoparticles embedded in a silica matrix: from spherical to prolate shape. Nanoscale Res Lett 2011, 6: 55. doi:10.1186/1556-276X-6-155
- Mieskes HD, Assmann W, Gruner F, Kucal H, Wang ZG, Toulemonde M: Electronic and nuclear thermal spike effects in sputtering of metals with energetic heavy ions. Phys Rev B 2003, 67: 155414–155425. doi:10.1103/PhysRevB.67.155414View Article
- Beuve M, Stolterfoht N, Toulemonde M, Trautmann C, Herbert Urbassek HM: Influence of the spatial and temporal structure of the deposited-energy distribution in swift-ion-induced sputtering. Phys Rev B 2003, 68: 125423–125428. doi:10.1103/PhysRevB.68.125423View Article
- Ziganshina SA, Bukharaev AA, Shamsetdinova LI, Chuklanov AP, Bizyaev DA: Atomic force microscopy of cobalt nanoparticles with electro-catalytic properties. J of Surf Invstgn: X-ray, Synch and Neut Tech 2009, 3: 725–729. doi:10.1134/S1027451009050115/View Article
- Sprouster DJ, Giulian R, Araujo LL, Kluth P, Johannessen B, Cookson DJ, Ridgway MC: Swift heavy-ion irradiation-induced shape and structural transformation in cobalt nanoparticles. J Appl Phys 2011, 109: 113504–113510. doi:10.1063/1.3587171View Article
- Agarwal G, Jain A, Agarwal S, Kabiraj D, Jain IP: Structural and electrical properties of swift heavy ion beam irradiated Co/Si interface. Bull Mater Sci 2006, 29: 187–190. doi:10.1007/BF02704614View Article
- Agarwal G, Sharma P, Jain A, Lal C, Kabiraj D, Jain IP: Ion beam induced mixing at Co/Si interface. Vacuum 2009, 83: 397–400. doi:10.1016/j.vacuum.2008.05.016View Article
- Lowes TD, Zinke-Allmang M: Cobalt grain growth on clean Si(100) surfaces. Scanning Microsc 1998, 12: 119–127.
- Particle interactions with matter [http://www.srim.org] 
- Pelletron Accelerator RBS-AMS Systems (PARAS) [http://iuac.res.in/accel/paras] 
- Toulemonde M, Dufour C, Paumier E: The ion–matter interaction with swift heavy ions in the light of inelastic Thermal Spike Mode. Acta Phys Pol A 2006, 109: 311–322.
- Toulemonde M, Costantini JM, Dufour C, Meftah A, Paumier E, Studer F: Track creation in SiO2 and BaFe12O19 by swift heavy ions: a thermal spike description. Nucl Instrum Methods B 1996, 116: 37–42. doi:10.1016/0168–583X(96)00007–9 10.1016/0168-583X(96)00007-9View Article
- Mookerjee S, Beuve M, Khan A, Toulemonde M, Roy A: Sensitivity of ion-induced sputtering to the radial distribution of energy transfers: a molecular dynamics study. Phys Rev B 2008, 78: 045435–045445. doi:10.1103/PhysRevB.78.045435View Article
- Srivastava SK, Avasthi DK, Assmann W, Wang ZG, Kucal H, Jacquet E, Carstanjen HD, Toulemonde M: Test of the hypothesis of transient molten state diffusion for swift-heavy-ion induced mixing. Phys Rev B 2005, 71: 193405–193408. doi:10.1103/PhysRevB.71.193405View Article
This article is published under license to BioMed Central Ltd. This is an open access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.